198 
Intensity | 
of Magnet- 
ization. 
Temperature 346°38. 
Tal 
102°8 
104°5 
131-2 
1462 
158°9 
188°0 
210°7 
224-0 
235°8 
244-0 
“1D He 
Or 
H= QOIS 1D ee 
H= Ot 1S A109 S OD 
Cr TW DW Wwst1Oor Ke 
Per- 
201°8 
202°7 
185°9 
186°3 
1750 
150-4 
133'8 
120-0 
1166 
84:3 
70°0 
Dr. Harrison on Variation with Temperature of 
Table I.—WNickel. 
| 5 
| Intensity 
mneability. | of Magnet- 
ization. 
Set I. (cont.). 
8-4 
535 
69°4 
83°57 
| 88°58 
100°3 
1170 
133°8 
152°1 
160-4 
167°14 
173°9 
Temperature 361°°25. 
Per- 
meability. 
1192 
109°98 
1193 
114-9 
110°2 
pe het 
95:5 
86°9 
765 
599 
50°1 
Temperature 371°°7. 
PS Ga 
PIA Oe 
HS CO He Go Go 
TaBLE I].— Nickel. Set II. Annealed at 600°. 
Intensity 
of Magnet-| 
ization. 
“I bo 
DOW WAGS 
Ot 
| 
18:47 
24°98 
28°92 
32°42 
28°56 
28°49 
| Magnetizing | Pees | 
0 | meability. 
Intensity 
of Magnet- 
ization, 
‘Temperature 17°. 
| 
Temperature 993. 
Per- 
meability. 
¥ 
: 
~ 
i 
‘ 
, 
d 
